上镀剂再次冲洗工件表面，确保电镀前表面没有生锈。干燥提高了铁片的温度，避免了铁片表面水分过多，在电镀时爆轰。热锌锌工件在440 -470 c的熔融锌溶液中浸泡，经过一定时间后，在铁艺工件表面形成一层锌铁合金层和纯锌涂层。
双顿罗庄罗庄护栏 咨询热线：0536-8695001 www.hulan800.com
Before pickling, check and check whether there are galvanized process holes in iron workpieces in our factory (exhaust, zinc entry, hanging), whether the iron on the surface of the workpieces with corrosive degree, and whether the surface coverage can be hydrochloric acid (such as paint, grease, etc. should be fired, ground, alkali cleaned, etc.).
Degreasing (alkali washing) equipment heating equipment to remove grease and paint on the surface of iron block. Wash off the alkali water and accessories on the surface of the iron block. The surface of rust and oxide is removed by pickling.
After pickling, inspection and treatment: whether the pickling effect is ideal, such as inadequate pickling, then pickling, if the pickling before treatment is not complete, need pickling back. Clean acidic water and other attachments on the surface of iron blocks.
The surface of the workpiece is washed again with the plating agent to ensure that there is no rust on the surface before plating. Drying improves the temperature of iron sheet, avoids excessive moisture on the surface of iron sheet, and detonates during electroplating. Hot zinc and zinc workpieces were immersed in 440-470 C molten zinc solution. After a certain period of time, a zinc-iron alloy layer and a pure zinc coating were formed on the surface of iron workpieces.
Passivation can make the surface of the workpiece corrosion resistant and reduce or prolong the occurrence time of white rust. Cooling prevents collective structure cracking after quenching. Zinc nodules and zinc powder were coated on the surface of the coating.
Shuangdun Fence Consulting Hotline: 0536-8695001 www.hulan800.com